Microwave spin resonance investigation on the effect of the post-processing annealing of CoFe2O4 nanoparticles

A novel investigation on the finite-size effects on the spin resonance properties of cobalt ferrite (CoFe2O4) nanoparticles has been performed using a room temperature ferromagnetic resonance (FMR) technique. A single broad spectrum was obtained for the CoFe2O4 nanoparticle samples, which indicated that all the samples were showing ferromagnetic characteristics. An asymmetric FMR line shape with a hefty trailing section was obtained due to the high magneto-crystalline anisotropy in CoFe2O4 nanoparticles, which changed with the size distribution. The resonance field for the samples shifted to a higher value due to the increase in the magneto-crystalline anisotropy in the CoFe2O4 nanoparticles with an increase in size. A systematic change in the resonance field and line width was observed with the change in the size distribution of the particles. Initially, it decreased with an increase in the size of the particles and increased after the critical size range. The critical size range is the imprint of the shift of the magnetic domain from a single domain to multi domain. The line width increased at higher annealing temperatures due to the enhancement in the dipole–dipole interaction, which led to a higher spin concentration as well as magneto-crystalline anisotropy. Furthermore, the saturation magnetization (Ms) as well as ‘Mr/Ms’ increased from 37.7 to 71.4 emu g−1 and 0.06 to 0.31, respectively. The highest coercivity (750.9 Oe) and anisotropy constant (4.62 × 104 erg cm−3) were found for the sample annealed at 700 °C, which can be corroborated by the literature as the critical annealing temperature at which CoFe2O4 nanoparticles shift from single domain nanoparticles to multi-domain nanoparticles. Post-processing annealing is critical in advanced processing techniques and spin dynamics plays a vital role in various interdisciplinary areas of applications.


Introduction
In recent years, the evolution of electromagnetic radiation sources has undergone exponential advancement that is re-ected in the increase in electromagnetic interference (EMI) shielding research, which is one of the key applications of magnetic nanoferrites. [1][2][3][4][5] The nanocrystalline ferrites have been a subject area of immense potential due to their profound applications in a wide range of interdisciplinary areas such as magnetic resonance imaging, drug delivery, magnetic hyperthermia treatment, spintronics, high-density memory devices, microwave devices, and power transformers. 2,6-10 To achieve a higher gure of merit in these applications, the properties of magnetic nanoparticles (MNPs) need to be optimized for relevant applications.
Ferrites belonging to the AB 2 O 4 group (family) are mainly controlled by divalent cations, which occupy the tetrahedral 'A' sites, and trivalent cations, which have a high degree of affinity for the octahedral 'B' sites. 11,12 Therefore, the whole range of distribution of cations possible in spinel ferrites can be shown by the general formula (M 1Àa 2+ Fe a 3+ ) [M a 2+ Fe 2Àa 3+ ], where cations inside the round and square brackets occupy the tetrahedral and octahedral sites, respectively. Alpha (a) represents the degree of inversion and shows the fraction of the tetrahedral site occupied by Fe 3+ cations, which depends on the synthesis method and post-annealing. If a ¼ 0, the spinel ferrite is normal; when a ¼ 1, it is an inverse spinel ferrite. However, if 0 < a < 1, the spinel ferrites are mixed. 7 The presence of two transition metal ions at the crystallographic site leads to a unique type of hopping conductivity and magnetic coupling. CoFe 2 O 4 is an interesting material because of its high magnetocrystalline anisotropy, coercivity, chemical stability, good a CSIR-National Physical Laboratory, New Delhi, India-110012. E-mail: rppant@ nplindia.org; prashantkhichi92@gmail.com electrical insulation, mechanical hardness and moderate magnetization at room temperature. 12,13 Apart from this, CoFe 2 O 4 has excellent physical and chemical stability, which makes it suitable for magnetic recording applications as highdensity digital recording disks. A recent investigation has shown that the cobalt ferrite nanoparticles have photo-induced magnetic properties. 14 Magneto-crystalline anisotropy is a very important parameter in connection with the characterization of the materials utilized in technical applications, particularly magnetic recording media. Magneto-crystalline anisotropy strongly depends on the interaction of cations in the A and B sites, which can also be altered by changing the latticeoccupancy state, crystallite size, bond angle and bond length. 7 Pure and doped CoFe 2 O 4 show a variety of novel properties that vary with the nature of the cations, their charge and site occupancy distribution between tetrahedral and octahedral sites. 7,11,15,16 Different experimental methods have been used in the preparation of ferrite nanoparticles such as sol-gel techniques, 13 co-precipitation, 1,17 hydrothermal, 18 microemulsion 19 and combustion methods, 20 etc. Among all of these, the coprecipitation method has been widely used as the prepared sample exhibits high crystallinity, homogeneity and good textural properties of the obtained material. 1,7,17 Also, this technique offers an advantage due to its low cost, high-quality production and less time consumption.
Also, the magnetic properties of the CoFe 2 O 4 nanocrystals depend on the different sizes, shapes and synthesis methods. 20,21 C. H. Chia et al. prepared a series of CoFe 2 O 4 nanocrystalline powders with varying synthesis temperatures and further annealing was done at different temperatures to optimize the structural and magnetic properties using the chemical co-precipitation method. 17 They reported a signicant increase in the saturation magnetization (M s ) from 43.2 to 60.7 emu g À1 , with the annealing temperature from 300 to 1200 C. A similar trend was also found in the coercive eld (H c ), which increased from 376 Oe at 300 C to 1201 Oe at 1200 C. However, the coercive eld H c reached its maximum of 1373 Oe at 400 C and then decreased to 870 Oe at 600 C. 22 The drastic change in H c for high-temperature annealed samples (900 C) might originate from the transition of a single magnetic domain to a multi-domain within a particle. Further, K. Rana et al. 12 synthesized CoFe 2 O 4 magnetic nanoparticles using the citrate precursor method and post-processing by annealing was done in the temperature range 700-1100 C. They suggested that the increase in the crystallite size and magnetization was due to the increase in the annealing temperature. Also, the M s and coercive eld increased from 53.69 to 74.46 emu g À1 and 257.40 to 304.99 Oe, respectively. A linear increase in the saturation magnetization (M s ) with the annealing temperature was observed in CoFe 2 O 4 MNPs, although the M s values of the samples were signicantly lower than the bulk value of 90 emu g À1 . 12 Even though numerous methods have been reported extensively for the CoFe 2 O 4 preparation, the precise control of the size and morphology to achieve desired properties is still in progress. The investigation of spin dynamics plays a key role in the EMI shielding operation and has been reported for the CoFe 2 O 4 by many researchers. However, most of the research reports limit their discussion to the resonance eld and g-value, which are major imprints of the material characteristics. 7,15,23 Other key spin resonance parameters that can provide a more detailed understanding of the properties of materials required to enhance the performance of the device have rarely been reported in the literature. 7 In the present work, CoFe 2 O 4 MNPs were synthesized by a wet chemical co-precipitation method and post-processing was carried out by annealing the as-prepared CoFe 2 O 4 powder at different temperatures (300-900 C). A detailed investigation of the microwave resonance behaviour was carried out by a ferromagnetic resonance (FMR) study and the spin resonance parameters were calculated by tting the FMR spectra. The present study emphasizes the modication of the structural, morphological, static and dynamic magnetic properties of the single-phase cobalt nanoferrites by postprocess annealing.

Synthesis
CoFe 2 O 4 ferrite nanoparticles were synthesized by a wet chemical co-precipitation method having the stoichiometric ratio of Co/Fe equal to 1 : 2. High-purity chemical precursors FeCl 2 -$4H 2 O, CoCl 2 $4H 2 O and NaOH (99.99%, from Sigma Aldrich) were used without further purication. The 0.23 M iron chloride (FeCl 2 $4H 2 O) and 0.16 M cobalt chloride (CoCl 2 $4H 2 O) solutions were prepared in DI water and heated to 80 C under constant stirring for 2 hours; the pH was maintained at 10 using 8 M ammonium hydroxide (28%) solution. The precipitated particles were centrifuged at 5000 rpm followed by washing several times with ethanol and DI water to obtain a uniform and narrow size distribution of particles. The obtained precipitate was then ltered and dried overnight in the oven at 70 C to remove the water content. Finally, the black powders of CoFe 2 O 4 were ground into ne powder and annealed at four different temperatures: 300 C (sample-a), 500 C (sample-b), 700 C (sample-c), 900 C (sample-d) in an argon (Ar) gas atmosphere for 3 hours with a slow heating rate of 5 C min À1 and then cooled down to room temperature under the same conditions. The nal obtained annealed black powders were used for the different characterizations to study the annealing effects on the material properties.

Characterization
The X-ray diffraction (XRD) patterns of the powder samples of magnetic nanoparticles were obtained with a multipurpose Xray diffractometer (Rigaku Ultima-IV). The diffraction pattern was recorded at a tube voltage and current of 40 kV and 30 mA, respectively, using Cu-Ka (l ¼ 1.54056Å) radiation with the scan step size of 0.02 and a scan speed of 2 min À1 in the 2q range from 20 to 80 . The average crystalline size was estimated by the Debye-Scherrer equation and the Williamson-Hall method. The X-ray diffraction (XRD) patterns of the samples were probed by employing the Rietveld renement technique using the Full Prof soware, which is a well-established technique for evaluating the structural parameters from powder diffraction data. The Rietveld method is a well-established technique for extracting structural details from powder diffraction data. The method employed a least-squares procedure to compare the Bragg intensities and those calculated from a possible structural model. The pattern renement was achieved in the following two steps: the background removal and scaling by the evaluation of structural parameters and site occupancies. The morphologies of the samples were studied using a high-resolution transmission electron microscope (HRTEM), model TECNAI F30. The specimens were prepared by sonicating the powdered sample dispersed in ethanol for about 30 min, followed by a uniform disperse solution dropped on the 300 mesh copper grid and dried at room temperature. Further, the size distribution of the samples was studied using smallangle X-ray scattering (SAXS) by tting the SAXS plot, assuming normal log distribution. The Fourier transform infrared (FTIR) spectra were recorded with a NICOLET 5700 set up in the range 400-2500 cm À1 . The dried samples were mixed with a KBr matrix and the spectra were recorded in the transmission mode. The room temperature magnetic measurements were carried out by using a vibrating sample magnetometer (model Lakeshore 7410 VSM). The room temperature microwave resonance study was performed using a Bruker EMX-10 spectrometer with a 100 kHz modulation eld. The measurements were performed using X-band (9.85 GHz) frequency in a rectangular cavity. 2,2-Diphenyl-1-picrylhydrazyl (DPPH) was used as the standard sample to validate the experimental results.

Results and discussion
3.1 Structural study using XRD Fig. 1(i) shows the XRD patterns of the different annealed samples (a, b, c, d) and their Rietveld renements are shown in Fig. 2. The Rietveld renement was carried out using the FULLProf-suite soware for the measured X-ray diffraction data of each annealed sample. All the diffraction peaks are in good agreement with the cubic spinel phase of CoFe 2 O 4 ferrite, consistent with JCPDS card no. 22-1086. 12 The rened prole c 2 was observed in the range 1.08 to 1.90, which is in very close proximity and evidences the existence of a single-phase cubic spinel ferrite structure with Fd3m (227) symmetry. 24 The crystallite size and strain were calculated using the Debye-Scherrer The variations in crystallite size as obtained from the Debye-Scherrer and Williamson-Hall methods and lattice parameters as obtained from Le Bail renement are summarised in Table 1, showing the difference in the values of the lattice parameters of the annealed samples. At higher annealing temperatures, the lattice parameter and crystallite size increased, and a similar trend has also been observed in another study aer annealing. 1 The growth of the crystallite size at higher annealing temperature could be because the solid-vapour surface of the crystal was replaced by a solid-solid interface via diffusion, which reduced the overall surface energy during the thermal annealing and caused the expansion of the crystallite volume. 20,27 However, the strain, Xray density and specic surface area were decreased with the increase in annealing temperature (Table 1), which could be related to the modication of the crystal structure and particle growth. 11 The calculated crystallite sizes of the annealed samples from both methods (Debye-Scherrer and Williamson-Hall plot), suggested the systematic increase in the crystallite size with the increase in annealing temperature, which is similar to an earlier report. 12 We calculated the specic surface area as per the following relation: Also, the X-ray density, r of the samples was calculated from the XRD patterns using the relation, r ¼ 8M/NV, where M is the molecular weight, N is Avogadro's number, and V is the cell volume. 7 Fig. 1-(ii) shows the variation in the lattice parameter and crystallite size with the increase in the annealing temperature. The variation in the specic surface area and particle size with annealing temperature is shown in Fig. 1-(iii). It can be seen clearly in Fig. 2 that the peaks became sharper for the sample with elevated annealing temperature, reecting the increased crystallite size.
The Le Bail renement of all the powder samples was performed using the pseudo-Voigt prole function. The values of all the renement parameters such as the "goodness of t" c 2 , the R factors (RP ¼ prole factor, RB ¼ Bragg factor, and RF ¼ crystallographic factor), lattice constant parameters (a, b, c), and the cell volumes (V) for all the samples were calculated, and the structural parameters obtained from prole renement are listed in Table 2.  The rened spectrum of each sample displayed a singlephase cubic spinel structure of CoFe 2 O 4 and the goodness of t was in the range of 1.08-1.90. The renement was carried out by assuming the Fd 3m symmetry (space group -227). Further, the renement was performed by xing the octahedral sites (16d (1/8, 1/8, 1/8)), tetrahedral sites (8a (1/2, 1/2, 1/2)) and free oxygen (32e (x, x, x)) sites. 7,11 The Rietveld renement depicts that the Le Bail t is optimum for extrinsic site transposal (g 0 ) equal 10% of the maxima. Moreover, the low g 0 value recommends the control of the size distribution of the CoFe 2 O 4 nanoparticle samples with no or very little intrinsic variations. The lattice parameters calculated by the renement and the position of oxygen atoms for each sample are plotted in Fig. 2(a-d). The complete process adopted for the Le Bail renement has been described in detail in our previous work. 7

FTIR analysis
FTIR is a very useful technique for deducing molecular dynamics and it gives information not only about the positions of divalent and trivalent metal ions in the spinel lattice, but also provides their vibrational modes. Fig. 3 shows the FTIR spectra for all the samples in the range 400-4000 cm À1 . In spinel ferrites, the IR spectral absorption bands are produced due to the vibrations of the oxygen ions with the cations present in the octahedral and tetrahedral sites in the unit cell. The characteristic region of interest for spinel ferrites is the absorptions in the 400-600 cm À1 range. 16 The high-frequency band n 1 is at around 500-600 cm À1 for M tetr -O and the low-frequency band n 2 is at around 400-490 cm À1 for M oct -O. Absorption bands observed within this limit reveal the formation of single-phase spinel structure having two sub-lattices, the tetrahedral (A) site and octahedral (B) site. 12 In this study, we observed the low-frequency band v 2 at around 412 cm À1 and the higher frequency band n 1 at around 554 cm À1 . The characteristic bands at 1368 cm À1 and 1550 cm À1 are due to the O-H bending peak, similar to the values obtained by Rana et al. 12 Also, the O-H stretching peak was observed at 3560 cm À1 as shown in Fig. 3. The reduction of the O-H diffraction peak with the increase in the annealing temperature is due to the loss of residual water molecules; we have observed that with the increase in the annealing temperature to 900 C, the peaks for water molecules were also diminished, and similar behaviour was also reported in literature. 12 As the annealing temperature increases, the intensities of the bands corresponding to O-H stretching vibrations decrease drastically, and this might be due to the loss of residual water molecules in all of the samples. 12,16 These band positions were found to be in agreement with the characteristic infrared absorption bands of cobalt ferrite nanocrystals because CoFe 2 O 4 is an inverse spinel in which Co 2+ ions occupy the octahedral sites and Fe 3+ ions occupy the tetrahedral sites. The absorption band n 1 is caused by the stretching vibrations of the tetrahedral metal (Fe 3+ )-oxygen bond, and the absorption band n 2 is caused by the octahedral metal (Fe 3+ /Co 2+ )-oxygen vibrations in octahedral sites. 21

Size distribution and morphology of samples using HRTEM and SAXS
The shapes and size distributions of the annealed magnetic nanoparticles were determined by HRTEM. In all the samples, the particles were found to be spherical with uniform size distribution. The average particle size was calculated from the TEM micrograph using Image-J soware; we used approximately 100 particles to plot the distribution for each sample as shown in Fig. 4. A gradual increase in the average particle size with the increase in annealing temperature was observed and is shown in Table 1. The increased average particle size could be due to the coalescence of crystallites at higher annealing temperatures. 20 The inset in Fig. 4 shows the high-resolution TEM images of ferrite nanoparticles exhibiting interplanar spacing values with their corresponding lattice planes. The inset HRTEM micrographs show the d-spacing of 0.29 nm, 0.25 nm and 0.20 nm, corresponding to the (220), (311) and (400) planes, respectively. The increase in the particle size obtained from the TEM is well in agreement with the crystallite size obtained from the Williamson-Hall method. Also, the other inset in Fig. 4 for different samples shows the obtained Selected Table 2 Rietveld refinement parameters of annealed CoFe 2 O 4 nanoparticles at 300 C, 500 C, 700 C and 900 C Sample  The size distribution was also measured by Small Angle X-ray Scattering (SAXS). Fig. 5 shows the plot between the distribution function and the particle size for all the samples. The size distributions of all the samples were obtained by tting the energy plot of the SAXS, assuming log-normal distribution and mean diameter. Fig. 5 depicts that sample 'a' has a narrow particle size distribution between 5-10 nm, which increased for sample 'b' to 5-20 nm, for sample 'c' to 2-35 nm and for sample 'd' to 10-70 nm; these are complementary to the TEM results. Sample 'a' depicts the le-skewed plot, which suggests that the particles in the sample are not spherical but are elongated along the X-axis. The SAXS plot obtained for samples 'b', 'c' and 'd' showed no skewness, conrming that the particles are spherical in nature. 25

Static magnetic measurement using VSM
The room temperature static magnetic measurements of all the samples were carried out with a magnetic eld up to 20 kOe. The magnetic hysteresis curves conrmed the ferromagnetic behaviour in all the annealed CoFe 2 O 4 nanoparticle samples. In general, the magnetization of the spinel ferrites depends on the distribution of the divalent and trivalent cations in the A and B sublattices of the unit cell. However, the total magnetic moment originated from the difference in the magnetic moments of the A (tetrahedral) and B (octahedral) sites, and therefore M s depends on the distribution of the cations. 7,20 The M-H loops of all annealed cobalt ferrite magnetic nanoparticles are shown in Fig. 6. Various magnetic parameters such as saturation magnetization (M s ), coercivity (H c ), remanent magnetization (M r ), anisotropy constant (k), etc. were calculated and are listed in Table 3. The anisotropy constant (k) was calculated using where H c is the coercivity, M s is the saturation magnetization, k is the anisotropic constant.   The M-H loops revealed the transition from the single domain to the multi-domain nature with the increase in the annealing temperature from 700 to 900 C, which led to an increase in the coercivity of sample 'c' and a decrease in the coercivity of sample 'd'. 21 The saturation magnetization (M s ) increased signicantly from 37.7 emu g À1 to 71.4 emu g À1 (Table 3) with the increase in annealing temperature from 300 to 900 C, showing the enhancement of ferromagnetism at a higher annealing temperature. The increase in the M s value for larger particle size was found at a higher annealing temperature, showing the dependence of M s on the particle size. 12 However, the coercivity increased gradually for the samples annealed at temperatures from 300 to 700 C and decreased on further increase in the annealing temperature to 900 C. This trend of change in the coercivity indicates the presence of the single domain nature in samples 'a', 'b' and 'c', and the multi-domain nature in sample 'd'. At 700 C the particle exhibited the single domain nature with the maximum value of coercivity among all the annealed samples because of the coherent rotation of spins, which is consistent with the literature. 17 The critical average particle size for the single domain was observed around 20 nm (sample c). The increase in coercivity from sample 'a' to sample 'c' (Table 3) could be attributed to the increase in the magnetic anisotropy for sample 'c'. 21,22 The magnetic anisotropy and coercivity decreased on increasing the annealing temperature to 900 C, due to the formation of the multi-domain region within the particles of sample 'd'. 1,28 The variation in the saturation magnetization and coercivity with particle size could also be explained on the basis of the magnetic domain structure, super-exchange interaction, particle diameter, magneto-crystalline anisotropy and shape anisotropy. 20 Combining all the magnetic properties of the annealed CoFe 2 O 4 nanoparticles, we can conclude that the saturation magnetization (M s ) value of the annealed samples increased up to 71.4 emu g À1 on increasing the annealing temperature up to 900 C, which is signicantly lower than the bulk CoFe 2 O 4 value of 90 emu g À1 . 12 Our results for M s are better at the nano-level and are higher than reported by Sajjia et al. (62 emu g À1 ). 13 The lower value of M s for nanoparticles could be attributed to the nite size effect. The nite-size effect shows a noncollinearity (spin canting) in the spinel structure (tetrahedral, A site, S A and octahedral, B site S B ) that results in a decrease in the net magnetic moment. 7,27,29 This is in accordance with the two-sublattice Néel model, dened as the difference between the moments of the A sublattice and B sublattice. The increase in the particle size favoured the increase in the collinearity of spins (S A and S B ) in the ferrimagnetic structure, which enhanced the saturation magnetization at higher annealing temperatures. The squareness ratio (R ¼ M r /M s ) was between 0.06-0.27, which decreased with an increase in the annealing temperature due to the decrease in the energy loss per unit cycle and its value was less than 0.5, so there was a uniaxial anisotropy according to the Stoner Wohlfarth model. 7,12 Also, for nano-sized ferrite particles, the surface area is larger and thus the surface energy and surface tension are higher as compared to the bulk.
Generally, in the collinear ferromagnetic (FiM) structure, the value of the magnetic moment per formula unit is calculated by considering the collinear two-sublattice Néel model of ferrimagnetism. In the present investigation, the calculated moment for each of the samples from the theory does not match the experimental values obtained from VSM. This discrepancy may be due to the spin canting at the B site; thus, we considered the three-sublattice Yafet-Kittel model to calculate the spin canting (basically a lack of full alignment of spins), which was already discussed in detail in our recent publication. 7 The canting angle f was calculated using the following assumption: M ¼ MB cos f À MA. The calculated values of the canting angles were 39.81, 32.44, 33.63 and 33.29 for the samples a, b, c and d respectively.
The schematic representation of the annealing effects on the domain structure of the CoFe 2 O 4 nanostructure is shown in Fig. 7. The schematic indicates that the increase in the particle size from 5-100 nm has two different domain wall structures. The annealed nanoparticles (300-700 C) were ferromagnetic with a single-domain nature, which converted to multi-domain particles upon annealing at 900 C.

Spin dynamics investigation using FMR
The spin dynamics of the magnetic nanoparticles have also been studied by performing ferromagnetic resonance (FMR) measurements. Fig. 8 shows the room temperature FMR spectra of samples (a, b, c, d) annealed at different temperatures. The resonance eld increased with the increase in the annealing temperature, which could be due to the change in the superexchange interactions between metallic ions through oxygen ions. Also, the lower magnetic moment of the smaller-sized sample increased the capability to attain the required splitting energy at lower magnetic eld values; the sample showed a resonance eld of 1057.72 G. With the increase in the annealing temperature, the resonance eld rst decreased to 721.54 G for sample b and then increased gradually to 1925.08 G for sample d. The FMR spectrum obtained for each sample was This journal is © The Royal Society of Chemistry 2020 Nanoscale Adv., 2020, 2, 1939-1948 | 1945 Paper Nanoscale Advances tted with different tting models (Lorentzian, pseudo-Voigt, and Gaussian) but the tting did not converge for any of the functions due to the asymmetric behaviour of the FMR line shape. Thus, to calculate DH PP , we divided the curve into two parts and the peak position of each curve was taken. The difference in the x-coordinate of the peak points represents the DH PP , which is used to calculate the spin resonance parameters. Further, we conrmed the values from the Win Acquisition soware by taking the peak position of the derivative curve, which is in close proximity. The decrease in the resonance eld (H r ) for sample 'b' can be attributed to the decrease in the line width (DH PP ) due to the stronger super-exchange interactions between the cations through the oxygen ions (Fe A ) at A-sites and B-sites. 23 The enhancement in the super exchange-interaction also increased the g-value for sample 'b' due to the magnetic ordering within each sublattice of CoFe 2 O 4 ferrite, which led to the rearrangement of cations at the A-site and B-site. 15 On annealing the nanoparticles at 700 and 900 C, the Co 2+ ions transferred from B-sites to A-sites, which caused the reduction in the super-exchange interactions between the metallic cations of spins at A-sites and B-sites through oxygen ((Fe A 3+ À O 2À À Fe B 3+ ) and (Co A 2 + ÀO 2À À Fe B 2 + )). The A-site is shared by both Fe 3+ and Co 2+ ions in these samples. Consequently, the resonance eld (H r ) and line width (DH PP ) increased, whereas the g-value decreased (see Table 4) at higher annealing temperatures (700 and 900 C). The reduction in the line width and enhancement in the g-value at higher temperature treatment of CoFe 2 O 4 ferrite was also observed in a previous study. 10 The increase in the peak to peak linewidth also indicated the enhancement in the dipole-dipole interactions in the CoFe 2 O 4 nanoparticles with the increase in the annealing temperature from 500 to 900 C. 30 The values of the spin resonance parameters are shown in Table 4. The spin concentration (N S ), as well as the peak to peak line width (DH PP ), signicantly depends on the annealing temperature. The dipole-dipole interactions and linewidth increased at higher annealing temperatures, resulting in higher N S . 30 The presence of the Co 2+ ions in CoFe 2 O 4 caused the high magneto-crystalline anisotropy of the material and broadened the FMR spectra. 10 Generally, N S is calculated by the comparison method with a standard DPPH, in which the area under the curve of DPPH (contains 1.52718 Â 10 18 spins per g) is compared with the area under the curve of the samples, provided all the conditions such as modulation amplitude, time constant and gain are the same. However, this method is not very reliable, so we calculated N S by statistical theory, which predicts that when the line shape is Lorentzian or between Lorentzian and Gaussian. The spin concentration can be calculated by the following equation: 7,31 Fig. 7 The effects of the annealing temperature on the domain structure of the nanoparticles.
where N S is in cm À3 and DH 1/2 is the linewidth (in Gauss) at half height of the absorption peak, DH 1/2 ¼ O3 DH PP , m B ¼ 9:274 Â 10 À 24 J T . The results obtained from the equation are given in Table 4. The asymmetric shape of the FMR spectra of samples 'c' and 'd' as shown in Fig. 8 could be related to the high anisotropy present in these samples. 32

Conclusions
Spin resonance phenomena and theory are of key importance for various applications. The FMR technique is a unique tool for investigating the spin dynamics behaviour of magnetic materials. In this work, we have investigated the spin dynamics in CoFe 2 O 4 samples of varying sizes by tting the FMR spectra with various theoretical models presented in the literature. There was a systematic variation in the spin resonance parameters such as resonance eld, g-value, spin concentration and line width. The spin resonance parameters were signicantly affected by the size distribution of the particles. The resonance parameters initially decreased with the size distribution and increased aer the critical size at which the material system changed from the single domain to the multi-domain. Broad FMR spectra were observed for all the samples with an asymmetric nature due to the high magneto-crystalline anisotropy. The structural and magnetic properties of annealed CoFe 2 O 4 magnetic nanoparticles have been discussed in detail. The experimental investigation revealed that annealing signicantly affects the physical and chemical properties of the CoFe 2 O 4 but no remarkable changes were observed in the crystalline phase of the particle. From the XRD results, we can conclude that the crystallite size increased from 5.9 to 39 nm at higher temperature annealing (300-900 C). The average particle size was increased from 10 nm to 41 nm on annealing the as-synthesized sample from 300 to 900 C, conrmed by TEM and SAXS studies, leading to a decrease in the specic surface area of the particle. Also, the strain factor was reduced for the particles annealed at a higher temperature. The formation of magnetic nanoparticles was conrmed by the presence of the lowfrequency band n 2 at around 412 cm À1 and the higher frequency band n 1 at around 554 cm À1 in the FTIR spectra. The static magnetic measurements revealed the transitions from the single domain to the multi-domain particles on annealing the sample at 900 C. The saturation magnetization M s value increased from 37.7 emu g À1 to 71.4 emu g À1 with the increase in the annealing temperature. The highest coercivity (750.9 Oe) and anisotropy constant (4.62 Â 10 4 erg cm À3 ) were observed for the sample annealed at 700 C. The wide FMR spectra revealed the ferromagnetic behaviour of CoFe 2 O 4 with a highly anisotropic nature and the resonance eld shied to a higher applied eld with an increase in the annealing temperature due to the increase in the dipole-dipole interaction. The characteristic bands at around 1368 cm À1 and 1550 cm À1 were due to the O-H bond. Also, the spin concentration of the samples increased at higher annealing temperatures. The small particle size ($10 nm) and good ferromagnetic properties present in the single-domain cobalt ferrite nanoparticles make them a promising candidate for biomedical applications to improve the quality of targeted drug delivery, magnetic resonance imaging (MRI) and hyperthermia treatment. The single-domain nanomagnetic particle having higher coercivity and moderate magnetization can be used for high-density magnetic storage applications, i.e. magnetic tape, hard disks, etc.

Conflicts of interest
There is no conicts of interest to declare.